caring for glazed architectural terra terra cotta was popular-ized in the late nineteenth century as...
Post on 17-May-2018
Embed Size (px)
Arthur L. Sanders, AIA, Senior Vice President and Director of Architecture, has over thirty years experience in the restoration of historic facade systems. Project Coordinator Kara L. Shypula, Assoc. AIA, provides investigation, document preparation, and construction administration services for building envelope projects.
Journal of architectural
technology published by
Hoffmann Architects, Inc.,
specialists in the rehabilitation
of building exteriors.
I S S U E 1 / 2 0 1 5 V O L U M E 3 2 N U M B E R 1
ne of the most prevalent materi-als found on historic buildings, glazed architectural terra cotta was popular-ized in the late nineteenth century as a versatile, lightweight, economical, and adaptable alternative to stone.
Through the 1930s, the sculp-tural properties of terra cotta gave rise to diverse archi-tectural styles, including the Chicago School, High Rise, and Beaux Arts styles.
Weighing roughly one-tenth as much as stone, architec-tural terra cotta is composed of kiln-baked clay called bisquea mixture of clay, previously fired clay products
(or grog), and waterwhich is finished with a protective glaze. Terra cotta can be molded and fired at high tempera-tures to a hardness and compactness comparable to that of brick. Readily shaped into sculptural forms, terra cotta offered designers an extensive
color palette and range of textures at a much lower cost than that of quar-ried stone.
After the 1871 Chicago fire, new building codes prompted specification of terra cotta as a lightweight, fire-resistant structural element in floor framing systems. Hollow structural terra cotta blocks were incorporated into fireproof construction in floors, walls, and ceilings. The 1930s saw the introduction of ceramic terra cotta veneer, in which terra cotta was cast as ceramic tile, attached to a grid of metal ties, and anchored to the build-ing as cladding.
Glazed architectural terra cotta is composed of hollow, hand-cast units, and adorns a number of noteworthy turn-of-the-century buildings, including the Woolworth Building in New York and the Wrigley Building in Chicago. As styles changed over time and pro-duction costs increased, terra cotta fell into disuse. In the late 1800s, there were over 100 terra cotta manufactur-ers in the United States; fewer than a dozen remain. The scarcity of qualified manufacturers and skilled craftspeople can present challenges to the ongo-ing maintenance and restoration of historic terra cotta.
When properly installed and main-tained, terra cotta is a durable, long-lasting material. Most significant
O Arthur L. Sanders, AIA and Kara L. Shypula, Assoc. AIA
Often finished in imitation of stone, terra cotta can be difficult to recognize and may be mistaken for cast stone, concrete, stone, or brick.
Caring for Glazed Architectural Terra Cotta
J O U R N A L
and thermal movement, and the ill ef-fects of improper repairs.
Water that penetrates between the clay bisque and finish glaze tends to migrate through the porous clay, lead-ing to disintegration of the terra cotta. One source of water entry might be delamination of the finish glaze, which can occur when the thermal coefficient of expansion between the clay and the glaze dont match. Alternatively, the original design may have supposed exaggerated water-proofing properties of the finish glaze, and systems for water management, such as flashings, weep holes, and drip edges, were never incorporated.
Cyclic wetting/drying and freezing/thawing can lead to glaze deteriora-tion, cracks and spalls in the body of the terra cotta, and fracturing and displacement of the units. Crazing, the formation of small random cracks in the glaze, occurs when the terra cotta unit absorbs moisture from the air and expands over many years. When new terra cotta is removed from the kiln, firing has shrunk it to its smallest size; over time, the porous clay grows, and the glaze goes into tension. Once the strength of the glaze has been ex-ceeded, it cracks and shatters, increas-ing the water absorption of the terra cotta unit and exacerbating water infiltration in a self-perpetuating cycle.
problems are due to inappropriate re-pairs, lack of maintenance, or both. By following good preservation practices, with attention to detail and workman-ship on par with the original design and craftsmanship, building owners and design professionals can achieve lasting restoration solutions to terra cotta deterioration.
Fabrication and Construction
Relatively inexpensive and highly adaptable, terra cotta was often used for ornamental detailing, and many historic buildings feature intricate sculptural terra cotta. Units are cast as hollow blocks, open at the back, with internal compartments, or webbing, that augment strength and loadbearing capacity without much added weight. For each type of unit, models are pre-pared, sized to accommodate shrink-age from drying and firing. A mold is then made from the model, and the clay is pressed against the inside of the mold. Alternatively, terra cotta may be extruded or ram-pressed.
Once the mold is removed, the unit is finished by hand and allowed to dry. The outer face is sprayed or brushed with glaze, typically a slip glaze / clay wash or an aqueous solution of metal salts. Not only does the glaze add color and finish effects, it creates a relatively impervious surface that protects the terra cotta from moisture
penetration. Historic glazes tended to be highly fade-resistant and durable. Once the glaze has been applied, the unit is fired in a kiln.
Finished terra cotta units were typical-ly installed with masonry backup and supported by steel lintels and angles. In early applications, bricks and mortar in the terra cotta cavities were some-times used to provide a connection with the masonry wall behind. After the turn-of-the-century, terra cotta construction typically employed metal anchors or wires set into the masonry backup and placed into preformed holes or slots in the terra cotta units.
Causes of Deterioration
Exposed and free-standing terra cotta detailing, such as balusters and parapets, tends to deteriorate more quickly than other facade elements. Where anchoring is extensive and complex, deterioration and failure likewise tend to be more pronounced. Deterioration to terra cotta used as load-bearing masonry tends to be less severe, owing to its simple or limited anchoring system, which presents fewer opportunities for corrosion-induced cracking and failure.
For most architectural terra cotta, deterioration may be traced to some combination of four basic factors: moisture infiltration, the resultant cor-rosion of embedded steel, structural
Failed prior repair effort. Crazed glazing. Crack and spall caused by corroded steel.
V O L U M E 3 2 N U M B E R 1
When water enters the wall system through poor detailing, insufficient maintenance, rising damp, a leaking roof, or other sources, the impervious glaze may impede moisture migra-tion and trap water inside the terra cotta unit. As temperature fluctuations increase pressure, sections of glazing or of the terra cotta itself may break off or spall. Glaze spalling tends to be-gin as blistering, when trapped water migrates to the surface and builds up pressure behind the glaze, eventually forcing pieces off the face of the unit. Glaze spalling may also be caused by corrosion of internal metal anchors.
When the terra cotta itself breaks apart or spalls, the result is a loss of visual integrity. With the porous un-derbody and anchoring exposed to the elements, the potential for water entry and further destructive effects increases.
Corrosion of Embedded Steel
As water penetrates, it comes in con-tact with embedded steel anchors and reinforcement. In historic applications, steel was often untreated, making it particularly susceptible to corrosion. As it corrodes, the steel expands, exerting pressure on the surrounding terra cotta and causing cracking and displacement. Embedded steel corro-sion may be caused by unmaintained roof drainage systems, which admit water into the cladding assembly.
What makes embedded steel cor-rosion challenging to treat is that it tends to be difficult to diagnose unless it is severe. By the time symptoms are visible at the surface, corrosion is likely already advanced. Initial outward signs of metal anchoring deteriora-tion might include staining and spalling. Total anchoring failure can result in loose terra cotta units, which are in danger of falling from the building.
Structural and Thermal Movement
Large cracks running through mul-tiple units or stories usually indicate problems with embedded structural elements. Rehabilitation often requires removal of pieces to examine and treat defects, such as corroded steel columns.
Most high-rise buildings from the early 1900s had little or no provisions for movement, so unaccommodated ther-mal expansion and contraction, along with building-frame shortening under load, placed sufficient strain on build-ing materials to cause displacement and cracking. Without proper expan-sion joints, buildings create their own, in the form of long cracks that admit significant water infiltration and invite further problems.
Many repairs fail prematurely because they do not address the root cause of distress or failure. Often, repair
materials are not durable and are incompatible with the existing terra cotta, creating a poor visual match and a short-term fix, at best. Where re-pairs fail, they tend to make deteriora-tion worse.
Poor detailing, including failure to properly anchor the patch to the backup, leads to failure of not only the r